Fluidity affects the minimum section thickness that can be cast, the maximum length of thin sections, fineness of feasibly cast details, and the accuracy of filling mould extremities. There are various ways of measuring the fluidity of a material, although it usually involves using a standard mould shape and measuring the distance the material flows. Fluidity is affected by the composition of the material, freezing temperature or range, surface tension of oxide films, and, most importantly, the pouring temperature. The higher the pouring temperature, the greater the fluidity; however, excessive temperatures can be detrimental, leading to a reaction between the material and the mould; in casting processes that use a porous mould material the material may even penetrate the mould material.The point at which the material cannot flow is called the coherency point. The point is difficult to predict in mould design because it is dependent on the solid fraction, the structure of the solidified particles, and the local shear strain rate of the fluid. Usually this value ranges from 0.4 to 0.8.An inclusion is a metal contamination of dross, if solid, or slag, if liquid. These usually are impurities in the pour metal (generally oxides, less frequently nitrides, carbides, or sulfides), material that is eroded from furnace or ladle linings, or contaminates from the mould. In the specific case of aluminium alloys, it is important to control the concentration of inclusions by measuring them in the liquid aluminium and taking actions to keep them to the required level.
There are a number of ways to reduce the concentration of inclusions. In order to reduce oxide formation the metal can be melted with a flux, in a vacuum, or in an inert atmosphere. Other ingredients can be added to the mixture to cause the dross to float to the top where it can be skimmed off before the metal is poured into the mould. If this is not practical, then a special ladle that pours the metal from the bottom can be used. Another option is to install ceramic filters into the gating system. Otherwise swirl gates can be formed which swirl the liquid metal as it is poured in, forcing the lighter inclusions to the center and keeping them out of the casting. If some of the dross or slag is folded into the molten metal then it becomes an entrainment defect. Metallurgical defects
There are two defects in this category: hot tears and hot spots. Hot tears, also known as hot cracking, are failures in the casting that occur as the casting cools. This happens because the metal is weak when it is hot and the residual stresses in the material can cause the casting to fail as it cools. Proper mould design prevents this type of defect.Hot spots are sections of casting which have cooled down more slowly than the surrounding material due to higher volume than its surrounding. This causes abnormal shrinkage in this region, which can lead to porosity and cracks.